This is an open access article published under a Creative Commons Attribution (CC-BY) License, which permits unrestricted use, distribution and reproduction in any medium, provided the author and source are cited.
Electroactive Nanoporous Metal Oxides and Chalcogenides by Chemical Design Christopher H. Hendon,†,‡ Keith T. Butler,‡ Alex M. Ganose,§,∥ Yuriy Roman-Leshkov,́ † David O. Scanlon,§,∥ Geoﬀrey A. Ozin,⊥ and Aron Walsh*,#,∇
† Department of Chemical Engineering, Massachusetts Institute of Technology, Cambridge, Massachusetts 02139, United States ‡ Department of Chemistry, University of Bath, Claverton Down, Bath, BA2 7AY, United Kingdom § Kathleen Lonsdale Materials Chemistry, Department of Chemistry, University College London, 20 Gordon Street, London, WC1H 0AJ, United Kingdom ∥ Diamond Light Source Ltd., Diamond House, Harwell Science and Innovation Campus, Didcot, Oxfordshire OX11 0DE, United Kingdom ⊥ Department of Chemistry, University of Toronto, Toronto, Ontario M5S 3H6, Canada # Department of Materials Science and Engineering, Yonsei University, Seoul 03722, South Korea ∇ Department of Materials, Imperial College London, Exhibition Road, London SW7 2AZ, United Kingdom
*S Supporting Information
ABSTRACT: The archetypal silica- and aluminosilicate-based zeolite-type materials are renowned for wide-ranging applications in heterogeneous catalysis, gas-separation and ion-exchange. Their compositional space can be expanded to include nanoporous metal chalcogenides, exempliﬁed by germanium and tin sulﬁdes and selenides. By comparison with the properties of bulk metal dichalcogenides and their 2D derivatives, these open-framework analogues may be viewed as three-dimensional semiconductors ﬁlled with nanometer voids. Applications exist in a range of molecule size and shape discriminating devices. However, what is the electronic structure of nanoporous metal chalcogenides? Herein, materials modeling is used to describe the properties of a homologous series of nanoporous metal chalcogenides denoted np-MX2, where M = Si, Ge, Sn, Pb, and X = O, S, Se, Te, with Sodalite, LTA and aluminum chromium phosphate-1 structure types. Depending on the choice of metal and anion their properties can be tuned from insulators to semiconductors to metals with additional modiﬁcation achieved through doping, solid solutions, and inclusion (with fullerene, quantum dots, and hole transport materials). These systems form the basis of a new branch of semiconductor nanochemistry in three dimensions.
1. INTRODUCTION The synthesis of ZSs is as challenging as it is important. In ﬁ ﬀ The concept of reconstructing a bulk semiconductor through the rst decade of this century, great e orts were expended to chemical synthesis into a semiconductor containing a periodic produce alternative zeolitic materials by replacing oxygen with 1 chalcogens and substituting the ubiquitous Si and Al with array of nanopores was introduced in 1992. The vision was a 4−6 new genre of semiconductor device with electronic, optoelec- alternate tetrahedral metal centers. Further structural tronic, and optical properties that were sensitive to the size and diversity including the isolation of metastable and unstable structureswas realized by application of structure directing shape of molecules adsorbed within the nanopores. The 7 archetypes of this class of zeolitic semiconductors (ZSs) were agents thereby expanding the structural library. Structurally, based on germanium and tin sulﬁde and selenide compositions. the incorporation of germanium allowed a proliferation of new They were found to have open-framework structures, frameworks and the synthesis of ultraporous framework 8,9 reminiscent of silica- and alumina-based zeolites, comprising materials. Moreover, the highly polarizable nature of tetrahedrally connected networks of tetrahedral metal chalco- chalcogen atoms was found to result in enhanced gas 10,11 genide building blocks.2 Inspired by this knowledge, their absorption in these systems. Latterly, alternative synthetic potential as electronic sensors was explored;3 however, information about their electronic structure, which is key to Received: February 6, 2017 establishing their physical structure, property, function, and Revised: March 27, 2017 utility relations, remains largely unknown today. Published: March 27, 2017
© 2017 American Chemical Society 3663 DOI: 10.1021/acs.chemmater.7b00464 Chem. Mater. 2017, 29, 3663−3670 Chemistry of Materials Article routes, such as ionothermal synthesis and post-synthesis arrangements because its large unit cell presented computa- reduction, have reinvigorated the search for new framework tional challenges for the heavier metal-chalcogenides. However, 12−15 structures and compositions. The recent report of the electronic properties of the ZSM-5-SiO2 were similar to that measured semiconducting behavior in a zeolite-analogue of ACO, SOD, and LTA. The electronic properties of the np- 16 material, as well as more exotic electronic phenomena such MX2 materials are essentially unperturbed by structure-type; as anomalous band gap evolution in nanocrystalline topological our computations on the smaller cell zeolites represent an insulators,17 shows that this ﬁeld oﬀers great potential. One upper limit in formation enthalpy. very recent study demonstrated the synthesis of open-frame The GeO2 frameworks display a similar stability with respect ﬁ 18 ZSM-5 high tin sul de and selenide zeolite analogues, with to the reference state than the SiO2 analogues with an enthalpic surface areas and stabilities equivalent or superior to zeolites. cost of 0.85 eV (SOD), 0.79 eV (LDA), and 0.84 eV (ACO), The conﬂuence of novel synthetic methods, early reports of respectively. The ability of germanium to form the same semiconducting behavior, and advances in modern computa- mineral structures as silicon can be understood from their tional techniques have inspired us to address the electronic similar ionic radii, electronegativities, and valence shell structure of these materials. characteristics.27 Indeed, large numbers of germanates that We report the electronic properties of nanoporous metal are isostructural to natural silicates have been synthesized. ﬀ − − chalcogenides (np-MX2, where M = Si, Ge, Sn, Pb; X = O, S, Some di erences exist between the Si O Si motif and the Se, Te) exempliﬁed by the sodalite (SOD), Linde Type A Ge−O−Ge motif,25 for example, the Ge−O bond is longer and (LTA) and aluminum chromium phosphate-1 (ACO) the germanate angle is smaller than the silicate species.28 The structures and compare these properties with those of the diﬀerence in bond length is related to ionic radius, while the bulk forms (MX2). The electronic structure is calculated from variation in bond angle can be understood in the context of the ﬁrst-principles within Density Functional Theory (DFT), a valence shell electron pair repulsion (VSEPR) model.29 In line predictive tool in contemporary materials design.19,20 We assess with VSEPR, there is a greater repulsion between nonbonded the nanoporous and bulk forms of the simplest metal electrons than bonded, thus the two nonbonded pairs force a chalcogenides, the corresponding metal oxides (np-MO2 and tighter angle in the bonding electrons in the germanate MO2) and mixed anion and cation solid solutions. The results structure. allow insights into how the structure and composition of There is an increase in formation enthalpy for the nanoporous metal chalcogenides determine their electrical and nanoporous sulﬁdes and selenides. As has been noted optical properties, and provide a robust platform for developing previously, the tilt angle joining the tetrahedral building blocks “inverse quantum dot” nanoporous semiconductors. of zeolite frameworks is largely ﬁxed at 109° in sulﬁde species,30 meaning that the formation of these frameworks involves 2. STRUCTURAL STABILITY additional strain, as reﬂected in the energies of Si, Sn, and Ge ﬁ Before we consider the electronic structure, it is pertinent to sul de and selenide species. The Pb chalcogenides and SiTe2 assess the stability of the phases. We emphasize that the represent a deviation from this trend. In these cases, the formation of most porous solids is kinetically controlled, with increased bond-lengths and higher atomic polarizability may be ﬂ nucleation and templating being key in the crystallization responsible for an enhanced exibility. For reference, the process. Nonetheless, the thermodynamic stability relative to formation enthalpies for all materials examined here are comparable to the formation enthalpy of other metastable known siliceous zeolites is an important comparison, which has 31 been made before to assess the viability of hypothetic materials (e.g., MOF-5). framework structures.21 It should be further noted that chalcogenide zeolitic frameworks are known, which consist of assemblages of First of all, all structures were found to be dynamically stable 32−35 with no negativity frequency phonon modes at the center of the nanoparticle building blocks of MX2 stoichiometry. This Brillouin zone. To address thermodynamic stability, we have is further suggested from our calculations; the one exception is calculated the total energies of the three framework types and the tellurides of which there are no reports in the solid-state compare them to the corresponding bulk crystal ground-state with a stoichiometry of MTe2. Given the predicted accessibility structures. The data is presented in Table S1. The pure silica of many of these species and other more strained ring 36 forms of ACO, SOD, and LTA are known to exist22,23 and can frameworks the existence of a plethora of experimentally be accessed through hydrothermal synthesis routes, employing realized analogues and the need for electronic insights to assist structure directing agents (SDAs or templates) as required. We in the realization of their true potential, we now undertake a ﬀ characterize the stability of the frameworks relative to the systematic exploration of the e ects of chemical and structural ﬁ ground-state crystal structure of the same stoichiometry by modi cations on the band-structure of these materials. calculating the energy diﬀerence per atom. For the ACO, SOD, 3. ELECTRONIC STRUCTURE and LTA frameworks of SiO2 the enthalpic cost associated with the formation of the porous solid is 0.55, 0.54, and 0.55 eV per The electronic properties of many porous materials feature formula unit, respectively. localization of the electronic density of states in real space and The SiO2-ZMS-5 material was also included in our energetic hence a lack of dispersion in the bands in reciprocal space. This assessment, as an industrially relevant material, and was found is certainly true for other porous materials (e.g., metal−organic to be highly stable with a formation enthalpy cost of 0.004 eV frameworks) in which many recent publications have shown ﬂat 37−39 per formula unit relative to SOD-SiO2. This stabilization is electronic bands in reciprocal space that can be modulated attributed to the reduction in acute M-O-M bonding angles. through chemical substitutions and inclusions.40,41 In the case These angles are critical descriptors in the assessment of of the porous metal oxides and chalcogenides presented here, stability of larger metal and chalcogenide-containing structures, the valence band is nondisperse (this is described by a large where more larger metal/chalcogenides favor more obtuse M- eﬀective mass for hole transport: m* >1m for np-SiO ), − h e 2 O-M angles.24 26 ZSM-5 was not studied in all compositional composed entirely of oxygen/chalcogen p-orbitals, independent
3664 DOI: 10.1021/acs.chemmater.7b00464 Chem. Mater. 2017, 29, 3663−3670 Chemistry of Materials Article
Φ Figure 1. Electronic band structures (DFT/HSE06), aligned to the vacuum level by the ionization potential ( ), of MO2 (M = Si, Ge, Sn, Pb) in the zeolite-type structures shown on the left. Plotted following 0,0,0 to 1/2,1/2,1/2 in reciprocal space (where 0,0,0 = gamma and 1/2,1/2,1/2 = special point as described in the ﬁgure), SOD structured materials show the most signiﬁcant dispersion in the conduction band (ca. 2 eV), followed by ACO (ca. 1.6 eV), and LTA (ca. 0.7 eV). The conduction band is composed of delocalized antibonding O s and M s-orbitals. The valence band is composed of localized O p-orbitals, resulting in ﬂat bands, and the bulk potential is relatively insensitive to the cation identity. of crystal morphology. These p-orbitals are orientated into the functions of np-MO2 semiconductors are relatively independent pores and thus do not form a continuous pathway in the of metal and morphology. This results from the similarities framework of the structure for charge transport; similar between the oxygen crystal environment−at the vertices of obstacles to hole mobility are often encountered in amorphous tetrahedra of M(IV) cations−and reﬂects the fact that the oxides.42 electron energies at these sites are dominated by the Madelung Owing to the stoichiometry and IV oxidation state of the potential.45,46 The electron aﬃnity (EA) is related to the energy group 14 metals Si, Ge, Sn, and Pb, the lowest unoccupied of the unoccupied metal center s-orbitals. The EA displays a states are a hybrid of unoccupied oxide/chalcogen and metal s- clear trend to increase as we move to larger metals, a trend orbitals. The crystal orbitals are delocalized throughout the related to the relativistic eﬀects of the nucleus on the electrons 2 ﬃ structure. As a result, np-MX2 materials demonstrate that scales with Z . This observed increase in electron a nity pronounced band dispersion (a parabolic eﬀective mass of may be attributed to a contraction in the s and p and expansion * me = 0.64 me for np-SiO2 in the SOD structure) comparable to of the d and f orbitals of the metal, resulting in stabilization of other wide band gap semiconductors.43 the low lying unoccupied states. The valence and conduction band edges are deﬁned by the To isolate the eﬀect of the anion, the electronic structure of chalcogen and metal/chalcogen identity, respectively (Support- the SnX2 series was explored, Figure 2. The ionization potential ing Information, Figure S1). These bands can be aligned to the (Φ) decreases with increase in anion size but only the oxide is 44 universal vacuum level: Figure 1 illustrates that the work predicted to have a band gap. Heavier np-MX2 compounds
3665 DOI: 10.1021/acs.chemmater.7b00464 Chem. Mater. 2017, 29, 3663−3670 Chemistry of Materials Article
observe a similar tendency toward a wider band gap with increased porosity, with LTA displaying the largest gap in all cases. Moreover, conduction band dispersion is aﬀected by nanoporosity, oﬀering a route toward the engineering of electron transport properties. For instance, the conduction ﬀ * band e ective mass me = 0.74 me for LTA-SiO2 compared to * me = 0.64 me for SOD-SiO2. Band engineering of solid-state semiconductors by creating solid solutions (compositional alloys) is a well-established practice. To consider the eﬀects of forming ZS alloys we treat two possible isovalent substitution routes for the SOD SiO2 framework: (i) a single extrinsic inclusion of another metal at the Si site; (ii) a single extrinsic chalcogenide substitution at an oxygen site. The results are summarized in Figure 3 (higher chalcogenide concentrations and energetics are presented in the Figure 2. Electronic band structures (plotted from 0,0,0 to 1/2,1/2,1/ Figure S4 and the Supporting Information, respectively). In 2 in reciprocal space) for sodalite SnX2 (X = O, S, Se, Te) relative to both the metal and the anion substitution cases, the band gaps the vacuum level. The oxide has a band gap, while the sulﬁde, selenide, ﬁ are intermediate between the binary end-points, that is, and telluride are metallic and their work functions are de ned by their ’ 48 Fermi levels (in the limit of T → 0 K). following Vegard s rule. The diﬀerent substitution types oﬀer precision control over which electronic property is tuned. The ionization potential can result in valence and conduction band crossing, thus forming a be altered by anion substitution, electron aﬃnity by metal semimetal (a zero gap material) with a low electronic density of mixing, and the band gap by either or both. In all cases the ﬁ states at the Fermi level. This is true of all np-MX2 materials, band engineering is achieved by introducing well-de ned states with the exception of SOD-SiS2 that has a predicted band gap in the gap of the host material. Doping on the chalcogen site of 0.2 eV. Further details of band alignments for np-MX2 are leaves the intrinsic band structure essentially unaltered and the provided in Table S1. resultant midgap state is highly localized, as evidenced by the Previous studies on nanostructured ZnO showed a large lack of dispersion in the upper valence band (Figure 3). Note eﬀect of the porosity of the material on the band gap.47 that the Te-substituted chalcogen resulted in a framework with − Although the magnitude of the band gap of IV VI np-MX2 a stress beyond the ultimate tensile strength of the framework materials is not as clearly modulated with morphology, we and could not be mechanically stabilized, although solid
Figure 3. Isovalent dopants introduce localized states in the electronic band structure of porous metal chalcogenides (DFT/HSE06), allowing for Φ ﬁ modular electronic band gaps and ionization potentials ( ). For example, in SiO2‑xSex (left-hand side), the low binding energy of the lled Se 4p orbitals introduces a state 2 eV above the valence of SiO2, while in Si1−xPbxO2 (right-hand side), the high binding energy of the unoccupied Pb 6s orbital introduces a state 3 eV below the conduction band of SiO2.
3666 DOI: 10.1021/acs.chemmater.7b00464 Chem. Mater. 2017, 29, 3663−3670 Chemistry of Materials Article solutions with heavier chalcogen frameworks (e.g., MSe2‑xTex) may be possible. The metal substitution induced gap state shows a trend toward increased localization as we move further in chemical space from the original host species. The dispersion for the Ge deﬁned conduction band is similar to that in purely siliceous SOD. The band dispersion in reciprocal decreases as we move down the column of the periodic table, until the ﬂat, midgap state of Pb. The trend can be understood in terms of atomic orbital mixing and overlap in forming the crystal wave functions. As the metals become more chemically distinct the degree of mixing is reduced and the state deﬁning the band edge participates to a lesser extent in the interconnected matrix of the framework. This observation has implications for charge transport in the material, as higher eﬀective masses will reduce electron mobility and hence conductivity.
4. SEMICONDUCTOR APPLICATIONS Thus far we have considered the properties of ZSs with respect to conventional solid-state semiconductors. However, the trends and properties that have been revealed are of interest in their own right, provoking the question: what is the nanoporous semiconductor advantage? The answer lies in the void, with the availability of a continuous, ordered, porous, conducting network. These systems can be intimately mixed with materials possessing complementary electronic properties. This concept opens up a plethora of combinations and opportunities. To illustrate the potential for forming composite systems we initially consider a prototypical pore-ﬁlling material: fullerene, ubiquitous in organic electronics. In combination with ZSs, we demonstrate Figure 4. Representations of (a) C60@LTA-SiO2 forming a type I how it can ﬁnd enhanced application. Figure 4 shows the upper semiconductor internal heterojunction, with strong quantum conﬁne- ment which could provide enhanced exciton lifetimes and valence electron density of LTA-SiO2 with a fullerene in the ﬀ pore,49 along with the associated electron energies, on the left- luminescence. The calculated o sets based on the isolated and composite systems are shown (blue bands corresponding to C60- hand side the energy levels. The straddling type-I offset of the ﬁ centered bands). SOD-SnO2 pores (d = 10.7 Å) may be lled with isolated materials is reproduced in the composite system. This small PbS quantum dots, where conﬁnement eﬀects can be exploited type of junction is widely applied in quantum dots and wells to to change the nature of the band oﬀsets. Here we show the broadening stabilize excitons and provide enhanced luminesce in the of the electronic gap in slightly larger PbS quantum dots and can conﬁned system. The arrangement means that both holes and project that the smaller dots will form the type-II semiconductor electrons are blocked from leaving the fullerene, yet the heterojunction. Loading ACO-GeO2 with the conductive polymer, fullerenes can still form an ordered array, aﬀorded by the polypyrrole (c), should form a type-III semiconductor heterojunction, framework structure of the ZS. We note that during the which could lead to selective hole transport in the polypyrrole layer preparation of this manuscript an exciting report of Ag and electron injection into the GeO2 framework. nanoparticles contained within zeolitic-SiO2 was reported and demonstrated unusual quantum conﬁnement eﬀects,50 sub- suited to acting as n-type semiconductors in such an stantiating this potential application. architecture, because of the greater dispersion and lower Type-II offsets or staggered band gaps alignment is perhaps eﬀective mass in the conduction band as opposed to the the most desirable alignment regime for semiconductor devices, valence. Design rules for p-type frameworks could include the ﬁnding application for example in bipolar transistors, light use of metal cations with lone-pair s-electrons constituting the emitting diodes, and photovoltaic devices. This type of oﬀset valence band maximum, similar principles have been explored allows for robust separation of charges (electrons and holes) for establishing p-type transparent conductive oxides.51 between the two materials. To illustrate the possibility of utility Type-III offsets usually occur in materials with contrasting of ZSs with other nanotechnologies we demonstrate the electronegativities, in this case the valence band of one material alignment of SOD-SnO2 with PbS quantum dots in Figure 4b. lies closer to the vacuum level than the conduction band of the In this case the size of the quantum dot as well as the porosity other material, resulting in a spontaneous transfer of charge at and composition of the framework allows for ﬁne-tuning of the the interface. Such architectures have been proposed for alignments. One application is the synthesis of photovoltaic biomedical applications; however, these oﬀsets are uncommon absorber layers with the high interfacial areas associated with in traditional semiconductors52,53 as the change in electro- bulk heterojunction solar cells but with a degree of order and negativity is generally accompanied by a large diﬀerence in regularity unobtainable in typical donor−acceptor composites. crystal structure. Recent developments in epitaxial growth of This in turn could lead to enhanced charge separation, carrier nanowires have opened up new possibilities for defect-free lifetimes, and ultimately device performance. For the type-III interfaces.54,55 The application of ZSs with semi- compositions considered here the frameworks would be best conducting inclusion materials oﬀers another route to the
3667 DOI: 10.1021/acs.chemmater.7b00464 Chem. Mater. 2017, 29, 3663−3670 Chemistry of Materials Article fabrication of this important class of semiconductor architec- exploited to stabilize late transition metal clusters via 63 tures. LTA-SiO2 with polypyrrole in the pore is depicted in encapsulation to generate bifunctional catalysts. Notably, Figure 4c. This case corresponds to a type-III oﬀset, with the the porous materials described herein can be synthesized with valence bands of the polypyrrole higher in energy than the tunable bandgaps, making them suitable as selective photoredox conduction band of the ZS, due to the destabilizing eﬀects of catalysts. Taken together, all these properties can be combined the lone pair on the nitrogen site. to address a variety of challenging transformations. For Another potential application of the frameworks is as example, these catalysts are promising materials for the selective transparent conductors (TCs). Traditionally TCs have relied removal of endocrine disruptor compoundswater-soluble on taking a wide gap material (usually an oxide) and tuning the organic pollutants known for their ability to mimic hormones, carrier levels to induce conductivity. Recently, however, Zunger leading to adverse health eﬀects on aquatic organisms64 and in and co-workers56 demonstrated a new route to achieving TCs the early stages of human life65 even at exceedingly low (i.e., through the control of interband transitions in metallic pg/L) concentrationsfrom wastewater streams via chemo- conductors. The proposed type 2 intrinsic conductors are selective photodegradation in the presence of other organic semimetals with large direct bandgaps and zero indirect species. Interestingly, the decomposition of organic waste could bandgaps. The SnX2 series presented in Figure 2 demonstrate lead to the production of fuels and electricity when using these how this kind of band structure is achievable in porous materials in photofuel-cells.66 Similar approaches could be chalcogenides. Through the choice of metal and anion the implemented for the removal of air pollutants in vehicles and interband transitions can be tuned to be symmetry allowed or buildings. Further, the cooperative eﬀects between the forbidden, suggesting the possible application of ZSs as semiconducting framework with encapsulated redox-active transparent intrinsic conductors. clusters can be exploited for light-assisted bond activation in The applications outlined above represent a select few thermocatalysis (an example is shown in Figure S3), akin to the examples; the ﬁeld is limited only by the imagination of its cooperative eﬀect attained with localized surface plasmons to practitioners. We have demonstrated the thermodynamic lower activation barriers and increase the selectivity by allowing feasibility of electroactive porous chalcogenide frameworks, the thermocatalytic production of sensitive compounds at lower and recent work in the ﬁeld of inﬁltrated carbon nanotubes57 temperatures.67,68 and electro-activated MOFs58 already demonstrates the wide array of novel technologies made possible by such strategies. 6. CONCLUSION The gauntlet is now thrown down to engineers to design and From a predictive materials modeling investigation, we have develop novel applications, to physicists to explore and explain shown that nanoporous oxides and chalcogenides exhibit an the rich electronic structure, and to chemists to synthesize and ﬁ impressive diversity in their electronic behavior. Depending on realize these con gurations. the choice of metal or chalcogen, the band gaps can be tuned 5. CATALYTIC APPLICATIONS from the regime of wide band gap insulators to semiconductors, with metallicity observed for the heavier chalcogens. Perhaps While the substitution of metallic heteroatoms into the these heavier chalcogenide materials could be interesting microporous matrix of zeolites has resulted in a large number electrically conductive materials. These properties can be of novel catalytic systems, the isomorphic substitutions of the further tuned through doping and solid solutions, and their bridging oxygen atoms in these materials by other elements, porosity can be exploited to construct a range of electronic such as S, Se, and Te, to produce microporous metal oﬀsets within the materials by using electroactive guests. The chalcogenides has seldom been explored and continues to be thermodynamic cost of forming the chalcogenide frameworks is 59 an exciting topic in the context of catalytic bond activation. similar to known nanoporous materials, and they should be This lack of understanding exists despite our ability to, on the amenable to the full range of established synthetic techniques one hand, synthesize well-deﬁned metal chalcogenide struc- including chemical templating. Furthermore, the diversity and tures, and on the other hand, use such materials with open chemical modularity provides unusual routes toward high architectures as catalysts in a variety of photo- and electro- surface area heterogeneous catalysts with compelling compo- 60 chemical applications. sitions for photo-, electro-, and thermal catalytic applications. An opportunity exists for the use of microporous metal Thus, this class of porous metal chalcogenides has the potential chalcogenides to generate exotic catalytic environments that to bring semiconductor nanochemistry ﬁrmly into three combine the conﬁnement eﬀects of microporous materials with dimensions. the electronic properties generated by the metal-chalcogen motifs. Indeed, microporous environments can discriminate ASSOCIATED CONTENT ﬀ ■ chemical pathways by allowing the di usion of molecules with * the correct shape and size. The pores and voids of these S Supporting Information materials have molecular dimensions capable of stabilizing The Supporting Information is available free of charge on the reactive intermediates and transitions states that mediate ACS Publications website at DOI: 10.1021/acs.chemma- chemical reactivity by van der Waals interactions. This is ter.7b00464. reminiscent of the solvation eﬀects prevalent within enzyme Further details on the computational methods and a table pockets and has analogous consequences for catalytic of the calculated electronic and structural properties of 61 speciﬁcity. The topochemical characteristics of the pores each material (PDF) mediate enthalpy−entropy compromises that determine Gibbs free energies of the reactive adducts, thus extending the AUTHOR INFORMATION diversity of the microporous solid matrix well beyond simple ■ size discrimination allowing the utilization of entropy as a Corresponding Author design principle.62 Microporous environments have been *[email protected].
3668 DOI: 10.1021/acs.chemmater.7b00464 Chem. Mater. 2017, 29, 3663−3670 Chemistry of Materials Article
ORCID (14) Jiao, F.; Jumas, J. C.; Womes, M.; Chadwick, A. V.; Harrison, A.; γ Christopher H. Hendon: 0000-0002-7132-768X Bruce, P. G. Synthesis of Ordered Mesoporous Fe3O4 and -Fe2O3 Yuriy Roman-Leshkov:́ 0000-0002-0025-4233 with Crystalline Walls Using Post-Template Reduction/Oxidation. J. − David O. Scanlon: 0000-0001-9174-8601 Am. Chem. Soc. 2006, 128, 12905 12909. (15) Hu, D.-D.; Lin, J.; Zhang, Q.; Lu, J.-N.; Wang, X.-Y.; Wang, Y.- Aron Walsh: 0000-0001-5460-7033 W.; Bu, F.; Ding, L.-F.; Wang, L.; Wu, T. Multi-Step Host−Guest Notes Energy Transfer Between Inorganic Chalcogenide-Based Semiconduc- The authors declare no competing ﬁnancial interest. tor Zeolite Material and Organic Dye Molecules. Chem. Mater. 2015, 27, 4099−4104. ■ ACKNOWLEDGMENTS (16) Lin, J.; Dong, Y.; Zhang, Q.; Hu, D.; Li, N.; Wang, L.; Liu, Y.; Wu, T. Interrupted Chalcogenide-Based Zeolite-Analog Semiconduc- A.W., K.T.B., and C.H.H. are supported by the Royal Society, tor: Atomically Precise Doping for Tunable Electro-/Photoelectro- the EPSRC (Grant EP/M009580/1) and the ERC (Grant chemical Properties. Angew. Chem. 2015, 127, 5192−5196. 277757). D.O.S. and A.W. acknowledge membership of the (17) Arachchige, I. U.; Kanatzidis, M. G. Anomalous Band Gap Materials Design Network. A.M.G. acknowledges Diamond Evolution from Band Inversion in Pb1‑xSnxTe Nanocrystals. Nano Lett. Light Source for the cosponsorship of a studentship on the 2009, 9, 1583−1587. EPSRC Centre for Doctoral Training in Molecular Modelling (18) Lin, Q.; Bu, X.; Mao, C.; Zhao, X.; Sasan, K.; Feng, P. and Materials Science (EP/L015862/1). GAO is a Government Mimicking High-Silica Zeolites: Highly Stable Germanium- and Tin- − of Canada Research Chair in Materials Chemistry and Rich Zeolite-Type Chalcogenides. J. Am. Chem. Soc. 2015, 137, 6184 Nanochemistry. He deeply appreciates the strong and sustained 6187. support of his research from the Natural Sciences and (19) Davies, D. W.; Butler, K. T.; Jackson, A. J.; Morris, A.; Frost, J. ﬁ M.; Skelton, J. M.; Walsh, A. Computational Screening of All Engineering Research Council of Canada. This work bene tted Stoichiometric Inorganic Materials. Chem. 2016, 1, 617−627. from access to the ARCHER, through the UK High (20) Butler, K. T.; Frost, J. M.; Skelton, J. M.; Svane, K. L.; Walsh, A. Performance Computing Consortium, which is funded by Computational Materials Design of Crystalline Solids. Chem. Soc. Rev. EPSRC Grant EP/L000202, and access to XSEDE Grant 2016, 45, 6138−6146. Number AC-1053575. (21) Zwijnenburg, M. A.; Bromley, S. T.; Foster, M. D.; Bell, R. G.; Delgado-Friedrichs, O.; Jansen, J. C.; Maschmeyer, T. Toward ■ REFERENCES Understanding the Thermodynamic Viability of Zeolites and Related (1) Ozin, G. A. Nanochemistry: Synthesis in Diminishing Frameworks through a Simple Topological Model. Chem. Mater. 2004, − Dimensions. Adv. Mater. 1992, 4, 612−649. 16, 3809 3820. (2) Han, C.; Sun, Q.; Li, Z.; Dou, S. X. Thermoelectric Enhancement (22) Corma, A.; Rey, F.; Rius, J.; Sabater, M. J.; Valencia, S. of Different Kinds of Metal Chalcogenides. Adv. Energy Mater. 2016, 6, Supramolecular Self-Assembled Molecules as Organic Directing Agent − 1600498. for Synthesis of Zeolites. Nature 2004, 431, 287 290. (3) Zheng, N.; Bu, X.; Wang, B.; Feng, P. Microporous and (23) Couves, J. W.; Jones, R. H.; Parker, S. C.; Tschaufeser, P.; Photoluminescent Chalcogenide Zeolite Analogs. Science 2002, 298, Catlow, C. R. A. Experimental Verification of a Predicted Negative 2366−2369. Thermal Expansivity of Crystalline Zeolites. J. Phys.: Condens. Matter − (4) Trikalitis, P. N.; Rangan, K. K.; Bakas, T.; Kanatzidis, M. G. 1993, 5, L329 L332. Varied Pore Organization in Mesostructured Semiconductors Based (24) Foster, M. D.; Rivin, I.; Treacy, M. M. J.; Friedrichs, O. D. A on the [SnSe ]4‑ Anion. Nature 2001, 410, 671−675. Geometric Solution to the Largest-Free-Sphere Problem in Zeolite 4 − (5) Bag, S.; Trikalitis, P. N.; Chupas, P. J.; Armatas, G. S.; Kanatzidis, Frameworks. Microporous Mesoporous Mater. 2006, 90,32 38. ’ M. G. Porous Semiconducting Gels and Aerogels from Chalcogenide (25) O Keeffe, M.; Yaghi, O. M. Germanate Zeolites: Contrasting the Clusters. Science 2007, 317, 490−493. Behavior of Germanate and Silicate Structures Built from Cubic T8O20 (6) Feng, P.; Bu, X.; Zheng, N. The Interface Chemistry between Units (T = Ge or Si). Chem. - Eur. J. 1999, 5, 2796−2801. Chalcogenide Clusters and Open Framework Chalcogenides. Acc. (26) Piccione, P. M.; Laberty, C.; Yang, S.; Camblor, M. A.; Chem. Res. 2005, 38, 293−303. Navrotsky, A.; Davis, M. E. Thermochemistry of Pure-Silica Zeolites. J. (7) Lewis, D. W.; Willock, D. J.; Catlow, C. R. A.; Thomas, J. M.; Phys. Chem. B 2000, 104, 10001−10011. Hutchings, G. J. De Novo Design of Structure Directing Agents for the (27) Goldschmidt, V. M. The Principles of Distribution of Chemical Synthesis of Microporous Solids. Nature 1996, 382, 604−606. Elements in Minerals and Rocks. J. Chem. Soc. 1937, 0, 655−673. (8) Jiang, J.; Jorda, J. L.; Diaz-Cabanas, M. J.; Yu, J.; Corma, A. The (28) Sastre, G.; Corma, A. Predicting Structural Feasibility of Silica Synthesis of an Extra-Large-Pore Zeolite with Double Three-Ring and Germania Zeolites. J. Phys. Chem. C 2010, 114, 1667−1673. Building Units and a Low Framework Density. Angew. Chem., Int. Ed. (29) Gillespie, R. J. The Valence-Shell Electron-Pair Repulsion 2010, 49, 4986−4988. (VSEPR) Theory of Directed Valency. J. Chem. Educ. 1963, 40, 295. (9) Corma, A.; Díaz-Cabañas, M. J.; Martínez-Triguero, J.; Rey, F.; (30) Li, H. Supertetrahedral Sulfide Crystals with Giant Cavities and Rius, J. A Large-Cavity Zeolite with Wide Pore Windows and Potential Channels. Science 1999, 283, 1145−1147. as an Oil Refining Catalyst. Nature 2002, 418, 514−517. (31) Hughes, J. T.; Navrotsky, A. MOF-5: Enthalpy of Formation (10) Armatas, G. S.; Kanatzidis, M. G. Mesoporous Germanium-Rich and Energy Landscape of Porous Materials. J. Am. Chem. Soc. 2011, Chalcogenido Frameworks with Highly Polarizable Surfaces and 133, 9184−9187. Relevance to Gas Separation. Nat. Mater. 2009, 8, 217−222. (32) Feng, P.; Bu, X.; Zheng, N. The Interface Chemistry between (11) Bag, S.; Kanatzidis, M. G. Chalcogels: Porous Metal− Chalcogenide Clusters and Open Framework Chalcogenides. Acc. Chalcogenide Networks from Main-Group Metal Ions. Effect of Chem. Res. 2005, 38, 293−303. Surface Polarizability on Selectivity in Gas Separation. J. Am. Chem. (33) Mohanan, J. L.; Arachchige, I. U.; Brock, S. L. Porous Soc. 2010, 132, 14951−14959. Semiconductor Chalcogenide Aerogels. Science 2005, 307, 397−400. 10‑ ’ (12) Santner, S.; Dehnen, S. [M4Sn4Se17] Cluster Anions (M = (34) Li, H.; Eddaoudi, M.; Laine, A.; O Keeffe, M.; Yaghi, O. M. Mn, Zn, Cd) in a Cs+ Environment and as Ternary Precursors for Noninterpenetrating Indium Sulfide Supertetrahedral Cristobalite Ionothermal Treatment. Inorg. Chem. 2015, 54, 1188−1190. Framework. J. Am. Chem. Soc. 1999, 121, 6096−6097. (13) Lin, Y.; Dehnen, S. [BMIm]4[Sn9Se20]: Ionothermal Synthesis (35) Luc, W.; Jiao, F. Synthesis of Nanoporous Metals, Oxides, of a Selenidostannate with a 3D Open-Framework Structure. Inorg. Carbides, and Sulfides: Beyond Nanocasting. Acc. Chem. Res. 2016, 49, Chem. 2011, 50, 7913−7915. 1351−1358.
3669 DOI: 10.1021/acs.chemmater.7b00464 Chem. Mater. 2017, 29, 3663−3670 Chemistry of Materials Article
(36) Zwijnenburg, M. A.; Cora,̀ F.; Bell, R. G. Dramatic Differences Buried N -Type CdO/P-Type SnTe Interfaces. Phys. Rev. B: Condens. between the Energy Landscapes of SiO2 and SiS2 Zeotype Materials. J. Matter Mater. Phys. 2015, 91, 205307. Am. Chem. Soc. 2007, 129, 12588−12589. (54) Pitanti, A.; Ercolani, D.; Sorba, L.; Roddaro, S.; Beltram, F.; (37) Butler, K. T.; Hendon, C. H.; Walsh, A. Electronic Structure Nasi, L.; Salviati, G.; Tredicucci, A. InAs/InP/InSb Nanowires as Low Modulation of Metal−Organic Frameworks for Hybrid Devices. ACS Capacitance N − N Heterojunction Diodes. Phys. Rev. X 2011, 1, Appl. Mater. Interfaces 2014, 6, 22044−22050. 11006. (38) Sun, L.; Hendon, C. H.; Minier, M. A.; Walsh, A.; Dinca, M. (55) Chen, C. Y.; Shik, A.; Pitanti, A.; Tredicucci, A.; Ercolani, D.; Million-Fold Electrical Conductivity Enhancement in Fe2(DEBDC) Sorba, L.; Beltram, F.; Ruda, H. E. Electron Beam Induced Current in − versus Mn2(DEBDC) (E = S, O). J. Am. Chem. Soc. 2015, 137, 6164 InSb-InAs Nanowire Type-III Heterostructures. Appl. Phys. Lett. 2012, 6167. 101, 63116. (39) Hendon, C. H.; Walsh, A. Chemical Principles Underpinning (56) Zhang, X.; Zhang, L.; Perkins, J. D.; Zunger, A. Intrinsic the Performance of the Metal−organic Framework HKUST-1. Chem. Transparent Conductors without Doping. Phys. Rev. Lett. 2015, 115, Sci. 2015, 6, 3674−3683. 176602. (40) McDonald, T. M.; Mason, J. A.; Kong, X.; Bloch, E. D.; Gygi, (57) Lim, H. E.; Miyata, Y.; Fujihara, M.; Okada, S.; Liu, Z.; Arifin; D.; Dani, A.; Crocella,̀ V.; Giordanino, F.; Odoh, S. O.; Drisdell, W. S.; Sato, K.; Omachi, H.; Kitaura, R.; Irle, S.; Suenaga, K.; Shinohara, H. Vlaisavljevich, B.; Dzubak, A. L.; Poloni, R.; Schnell, S. K.; Planas, N.; Fabrication and Optical Probing of Highly Extended, Ultrathin Graphene Nanoribbons in Carbon Nanotubes. ACS Nano 2015, 9, Lee, K.; Pascal, T.; Wan, L. F.; Prendergast, D.; Neaton, J. B.; Smit, B.; − Kortright, J. B.; Gagliardi, L.; Bordiga, S.; Reimer, J. A.; Long, J. R. 5034 5040. Cooperative Insertion of CO in Diamine-Appended Metal-Organic (58) Talin, A.; Centrone, A.; Ford, A. C.; Foster, M. E.; Stavila, V.; 2 Haney, P.; Kinney, R. A.; Szalai, V.; El Gabaly, F.; Yoon, H. P.; Frameworks. Nature 2015, 519, 303−308. Leonard,́ F.; Allendorf, M. D. Tunable Electrical Conductivity in (41) Park, S. S.; Hontz, E. R.; Sun, L.; Hendon, C. H.; Walsh, A.; Van Metal-Organic Framework Thin-Film Devices. Science 2014, 343,66− Voorhis, T.; Dinca, M. Cation-Dependent Intrinsic Electrical 69. Conductivity in Isostructural Tetrathiafulvalene-Based Microporous ́ − (59) Benz, S.; Lopez-andarias, J.; Mareda, J.; Sakai, N.; Matile, S. Metal-Organic Frameworks. J. Am. Chem. Soc. 2015, 137, 1774 1777. Catalysis with Chalcogen Bonds Communications. Angew. Chem., Int. (42) Wahila, M. J.; Butler, K. T.; Lebens-Higgins, Z. W.; Hendon, C. Ed. 2017, 56, 812−815. H.; Nandur, A. S.; Treharne, R. E.; Quackenbush, N. F.; Sallis, S.; (60) Regulacio, M. D.; Han, M. Multinary I-III-VI2 and I2-II-IV-VI4 Mason, K.; Paik, H.; Schlom, D. G.; Woicik, J. C.; Guo, J.; Arena, D. Semiconductor Nanostructures for Photocatalytic Applications. Acc. A.; White, B. E.; Watson, G. W.; Walsh, A.; Piper, L. F. J. Lone-Pair Chem. Res. 2016, 49, 511−519. Stabilization in Transparent Amorphous Tin Oxides: A Potential (61) Gounder, R.; Iglesia, E. The Roles of Entropy and Enthalpy in Route to P-Type Conduction Pathways. Chem. Mater. 2016, 28, Stabilizing Catalysis. Acc. Chem. Res. 2012, 45, 229−238. − 4706 4713. (62) Butler, K. T.; Walsh, A.; Cheetham, A. K.; Kieslich, G. (43) Hinuma, Y.; Hatakeyama, T.; Kumagai, Y.; Burton, L. A.; Sato, Organised Chaos: Entropy in Hybrid Inorganic−Organic Systems and H.; Muraba, Y.; Iimura, S.; Hiramatsu, H.; Tanaka, I.; Hosono, H.; Other Materials. Chem. Sci. 2016, 7, 6316−6324. Oba, F. Discovery of Earth-Abundant Nitride Semiconductors by (63) Na, K.; Choi, K. M.; Yaghi, O. M.; Somorjai, G. A. Metal Computational Screening and High-Pressure Synthesis. Nat. Commun. Nanocrystals Embedded in Single Nanocrystals of MOFs Give 2016, 7, 11962. Unusual Selectivity as Heterogeneous Catalysts. Nano Lett. 2014, 14, (44) Butler, K. T.; Hendon, C. H.; Walsh, A. Electronic Chemical 5979−5983. Potentials of Porous Metal-Organic Frameworks. J. Am. Chem. Soc. (64) Milla, S.; Depiereux, S.; Kestemont, P. The Effects of Estrogenic 2014, 136, 2703−2706. and Androgenic Endocrine Disruptors on the Immune System of Fish: (45) Born, M.; Huang, K. Dynamical Theory of Crystal Lattices; A Review. Ecotoxicology 2011, 20, 305−319. Clarendon Press, 1998. (65) Colborn, T.; Saal, F. S.; Soto, A. M. Developmental Effects of (46) Sallis, S.; Butler, K. T.; Quackenbush, N. F.; Williams, D. S.; Endocrine-Disrupting Chemicals in Wildlife and Humans. Enviromen- Junda, M.; Fischer, D. a.; Woicik, J. C.; Podraza, N. J.; White, B. E.; tal Heal. Perspect. 1993, 101, 378−384. Walsh, A.; Piper, L. F. J. Origin of Deep Subgap States in Amorphous (66) Viswanathan, B.; Subramanian, V.; Lee, J. S. Materials and Indium Gallium Zinc Oxide: Chemically Disordered Coordination of Processes for Solar Fuel Production; Lockwood, D. J., Ed.; Springer, Oxygen. Appl. Phys. Lett. 2014, 104, 232108. 2014. (47) Zwijnenburg, M. A.; Bromley, S. T. Structure Direction in Zinc (67) Linic, S.; Aslam, U.; Boerigter, C.; Morabito, M. Photochemical Oxide and Related Materials by Cation Substitution: An Analogy with Transformations on Plasmonic Metal Nanoparticles. Nat. Mater. 2015, Zeolites. J. Mater. Chem. 2011, 21, 15255−15261. 14, 567−576. (48) Vegard, L. Die Konstitution Der Mischkristalle Und Die (68) Boerigter, C.; Aslam, U.; Linic, S. Mechanism of Charge Raumfüllung Der Atome. Eur. Phys. J. A 1921, 5,17−26. Transfer from Plasmonic Nanostructures to Chemically Attached. ACS − (49) Hamilton, B. B.; Rimmer, J. S.; Anderson, M.; Leigh, D. White Nano 2016, 10, 6108 6115. Light Emission from C60 Molecules Confined in Molecular Cage Materials. Adv. Mater. 1993, 5, 583−585. (50) Fenwick, O.; Coutiño-Gonzalez, E.; Grandjean, D.; Baekelant, W.; Richard, F.; Bonacchi, S.; De Vos, D.; Lievens, P.; Roeffaers, M.; Hofkens, J.; Samorì, P. Tuning the Energetics and Tailoring the Optical Properties of Silver Clusters Confined in Zeolites. Nat. Mater. 2016, 15, 1017−1022. (51) Hautier, G.; Miglio, A.; Ceder, G.; Rignanese, G.-M.; Gonze, X. Identification and Design Principles of Low Hole Effective Mass P- Type Transparent Conducting Oxides. Nat. Commun. 2013, 4, 2292. (52) Butler, K. T. Morphological Control of Band Offsets for Transparent Bipolar Heterojunctions: The Badeker̈ Diode. Phys. Status Solidi A 2015, 212, 1461−1465. (53) Wahila, M. J.; Lebens-Higgins, Z. W.; Quackenbush, N. F.; Nishitani, J.; Walukiewicz, W.; Glans, P.-A.; Guo, J.-H.; Woicik, J. C.; Yu, K. M.; Piper, L. F. J. Evidence of Extreme Type-III Band Offset at
3670 DOI: 10.1021/acs.chemmater.7b00464 Chem. Mater. 2017, 29, 3663−3670